SRIVASTAVA, SHUBHAM. Numerical Simulation of Synthesis of One-Dimensional Molybdenum Oxide Nanostructures in Flame Environment. (Under the direction of Dr. Alexei Saveliev).
The past few decades have seen a great amount of interest in the field of nanotechnology. As
our world moves towards miniaturized devices nanotechnology is set to revolutionize the electronics, storage and sensing industry. Various methods for synthesis of different types of
nanoparticles are being explored. A few of these processes that hold great promise for the future are the flame synthesis methods. These methods are highly efficient but at the same time it is difficult to control the morphology of the produced nanoparticles due to a high
number of control parameters involved because of the complex flow processes. These issues demand a better understanding before these processes can be exploited to their maximum
Most numerical methods developed cater to the simulation of spherical nanoparticles.
However, it is now being increasingly understood that the shape and structure of a nanoparticle plays critical role in determining its chemical, physical and electronic properties. Therefore a high level of control on the shape of nanoparticles is highly
imperative. With this purpose in mind this work proposes a novel numerical scheme to simulate the synthesis of one-dimensional nanorods and further presents mathematical
simulations based on it followed by validation with experimental results.
have been coupled to each stage of nanoparticle development, namely monomer formation, nucleation, particle growth and particle transport. The numerical scheme takes into account
all the details of the complex surface phenomena taking place on a nanorod. Later, factors are studied which transition the growth characteristics of a nanoparticle from one dimensional to
a spherical structure, thus encompassing all the factors that influence the particle shape.
Group characteristics of nanoparticles have also been modeled by employing methods that track the growth of the entire set of nanoparticles in the flame volume. This gives a clear
picture of the growth of the particle ensemble in addition to the individual particles.
This work provides a first of its kind numerical model for one-dimensional growth of
Numerical Simulation of Synthesis of One-Dimensional Molybdenum Oxide Nanostructures in Flame Environment
A dissertation submitted to the Graduate Faculty of North Carolina State University
in partial fulfillment of the requirements for the degree of
Doctor of Philosophy
Raleigh, North Carolina 2014
_______________________________ ______________________________ Dr. Alexei Saveliev Dr. Tarek Echekki
Shubham Srivastava was born on 29th May 1984 in Agra, the city of the famous Taj Mahal,
in India. He obtained his Bachelor of Science degree in Mechanical Engineering from Manipal Institute of Technology, India in 2007. To advance his knowledge in Thermal
To begin with, I owe an enormous debt to Dr. Alexei Saveliev for giving me the opportunity
to undertake this research. His guidance, inspiration and patience have been a major contributing factor to the completion of this work. To him, I owe the vital learning from this
I would like to express my sincere gratitude to Dr. Tarek Echekki, Dr. Tiegang Fang, Dr. Kevin Lyons and Dr. Kazufumi Ito for serving as the co advisors in my defense committee.
Their valuable suggestions and advice were crucial for the completion of this manuscript. I am very thankful to my lab mates Parth, RC, Mengbai and Kundu for their support and
company. A special thanks to my roommates Tripathi Ji and Arun for all their help and for putting up with the mess of my papers and books in our house. Dileep, my friend and colleague, deserves a special mention for extending his generosity during my days of
Above all, I would like to express my heartfelt gratitude to my parents and family for all their
TABLE OF CONTENTS
LIST OF TABLES... ix
LIST OF FIGURES……… x
Chapter 1 Introduction ... 1
1.1 Definition of Nanomaterial and One-Dimensional Nanostructures... 1
1.2 Transition Metal Oxide Nanostructures ... 3
1.3 Flame Synthesis of Nanoparticles ... 5
1.3.1 Steps in Flame Synthesis of Nanoparticles ... 7
1.3.2 Parameters Affecting Flame Synthesis ... 9
1.3.3 Flame Synthesis of One-Dimensional Nanostructures ... 11
1.4 Numerical Modeling of Flame Synthesis of Nanoparticles ... 12
1.5 Thesis Objectives ... 14
1.6 Layout of the Thesis... 15
Chapter 2 Experimental Study ... 16
2.1 Experimental Set-up... 17
2.1.1 Thermophoretic Sampling Technique ... 18
2.1.2 Effect of Oxidizer Composition on the Flame ... 19
2.1.3 Effect of Strain Rate on the Flame ... 20
2.2 Experimental Results ... 21
2.2.1 Nanoparticle synthesis from 1.00 mm diameter molybdenum probe ... 22
2.2.2 Nanoparticle Synthesis from 0.75 mm Diameter Molybdenum Probe ... 26
2.3 Conclusions of Experimental Results ... 28
Chapter 3 Brief Introduction to the Numerical Model ... 30
3.1 Details of the Growth Model ... 32
3.2 Assumptions ... 33
Chapter 4 Flame Modeling ... 36
4.1 Opposed Flow Flame Model ... 37
4.2 Transport Properties ... 40
4.2.1 Mixture Averaged Properties ... 41
4.3 Solution Procedure ... 43
4.5 Results of the Flame Model ... 44
Chapter 5 Monomer Formation ... 50
5.1 Molybdenum Oxidation ... 51
5.2 Oxidation Regimes of Molybdenum ... 52
5.3 Mechanism of Molybdenum Oxidation ... 55
5.4 Rate Equation for Molybdenum Oxidation... 56
5.5 Calculation of Molybdenum Probe Temperature and Molybdenum Dioxide Concentration ... 60
5.6 Verification of the Molybdenum Oxidation Kinetic Model ... 61
Chapter 6 Nucleation ... 63
6.1 Classical Nucleation Theory (CNT) ... 65
6.1.1 Assumptions in CNT... 69
6.2 Lothe and Pound ... 69
6.3 Reiss, Katz and Cohen ... 71
6.4 On the Use of Classical Nucleation Theory in this Research ... 73
6.5 Verification of Implementation of Classical Nucleation Theory ... 74
6.5.1 Nucleation with varying temperature ... 75
6.5.2 Nucleation with varying supersaturation ratio ... 77
6.6 Conclusion for Nucleation Theory... 79
Chapter 7 Nanorod Growth Model ... 80
7.1 Rough Growth ... 81
7.2 Layered Growth ... 81
7.3 Growth Mechanism in Molybdenum Oxide Nanorods ... 84
7.3.1 Chemical Potential and Supersaturation Ratio ... 84
7.3.2 Phase Transition and Supersaturation Ratio ... 85
7.3.3 Variation of Growth Pattern with the Driving Force ... 87
7.3.4 Effect of Probe Diameter on Nanoparticle Morphology ... 88
7.4 Different Growth Modes on Nanorod Surfaces ... 89
7.5 Mechanism of Growth on Nanorod Tips ... 90
7.5.1 Direct Impingement ... 92
7.5.2 Diffusion of Atoms from Lateral Sides ... 94
Chapter 8 Particle Transport Model... 101
8.1 Drag... 103
8.1.1 Stokes’ Law ... 104
8.2 Thermophoretic Force ... 107
8.2.1 Theory ... 108
8.2.2 Thermophoretic Force in the Free Molecular Regime ... 108
8.2.3 Thermophoretic Force in the Continuum Regime ... 109
Chapter 9 Results of the Growth Model ... 112
Chapter 10 General Dynamic Equation Modeling ... 129
10.1 General Dynamic Equation ... 130
10.1.1 Sectional Methods ... 132
10.1.2 Monte Carlo Methods ... 133
10.1.3 Moment Methods ... 133
10.2 Method of Moments ... 134
10.2.1 Physical Significance of Moments... 134
10.2.2 General Dynamic Equation for Method of Moments ... 135
10.2.3 Restrictions to Method of Moments ... 136
10.2.4 Method of Moments with Interpolative Closure ... 137
10.3 Quadrature Method of Moments ... 138
10.3.1 Quadrature-Based Closure ... 139
10.3.2 Product Difference Algorithm ... 140
10.3.3 Verification of the Quadrature Method of Moments Algorithm ... 141
10.4 Quadrature Method of Moments Applied to Nanorod Synthesis ... 147
10.4.1 Growth ... 148
10.4.2 Nucleation ... 150
10.4.3 Particle Transport ... 151
10.4.4 Final Equations and Procedure for Quadrature Method of Moments ... 151
10.5 Results of Quadrature Method of Moments applied to Nanorod synthesis ... 153
Chapter 11 Conclusions ... 158
Appendix A: Derivation for Rate of Oxidation for Molybdenum...174
LIST OF TABLES
Table 5-1: Thermochemical data for Oxides of Molybdenum ... 53
Table 5-2: Classification scheme; oxidation of molybdenum (Gulbransen et. al., 1963) ... 54 Table 5-3: Comparison of calculated temperature of molybdenum probe to the experimental temperature….……… 62
Table 8-1: Values for various Cunningham corrections constants………106
LIST OF FIGURES
Figure 1-1: TEM images of BaTiO3 nanowires (Cao, 2004). ... 2
Figure 1-2: SEM images of ZnO nanobelts (Cao, 2004). ... 3
Figure 1-3: Transition metals shown on the periodic table (Wikipedia, 2014) ... 4
Figure 1-4: Different burner configurations (a) premixed flat flame burner (b) counterflow diffusion flame burner (c) coflow diffusion flame burner (Rosner, 2005) ... 6
Figure 1-5: Steps in particle formation in flames (Roth, 2007) ... 9
Figure 2-1: Schematic representation of the set-up (Desai, 2010). ... 17
Figure 2-2: Thermophoretic sampling technique (Merchan-Merchan, et al., 2003) ... 18
Figure 2-3: Methane flames at a strain rate of 20 s-1 formed by a) 21% O2, 79% N2 b) 50% O2, 50% N2 c) 100% O2 (Desai, 2010) ... 20
Figure 2-4: Flames at various strain rates (35% O2 + 65% N2): (a) SR = 10 s-1(b) SR = 20 s -1(c) SR = 30 s-1 (Desai, 2010). ... 21
Figure 2-5: Schematic of probe position (Desai, 2010). ... 22
Figure 2-6: Low resolution TEM image of nanoparticles collected at Z = 12 mm from the fuel nozzle (Desai, 2010). ... 23
Figure 2-7: TEM images of nanostructures obtained at Z = 10 mm from the fuel nozzle (Desai, 2010) ... 24
Figure 2-8: Magnified images of the nanoparticles sampled at Z = 10 mm (Desai, 2010). ... 25
Figure 2-10: Magnified TEM images of nanoparticles formed by 0.75 mm probe (Desai, 2010) ... 28
Figure 3-1: Subdivisions of the numerical model. ... 32 Figure 4-1: Schematic diagram of opposed flow diffusion flame. ... 37
Figure 4-2: Chemical species concentration profiles for counter-flow oxy-methane flame. . 46 Figure 4-3: Temperature of the flame. ... 47 Figure 4-4: Gas velocity as a function of axial position. ... 48
Figure 6-1: Distribution functions of embryos of different sizes according to Volmer and Becker-Doring theories of nucleation (Christian, 2002). ... 68
Figure 6-2 Comparison of all three theories to experiment (Hung, et al., 1989) ... 73 Figure 6-3: Rate of nucleation as a function of temperature at supersaturation ratios 5, 7, 10. ... 75
Figure 6-4: Size of critical nucleus vs Temperature for Supersaturation ratio = 10, 7, 5 ... 76 Figure 6-5: Rate of nucleation as a function of supersaturation ratio at T = 300, 400, 500 K 77
Figure 6-6: Size of critical nucleus vs saturation ratio at T = 300, 400, 500 K ... 78 Figure 7-1: 2D nucleation ... 83 Figure 7-2: Growth by screw dislocation (Venables, 1994) ... 83
Figure 7-3: Variation in crystal growth pattern with the driving force (Sunagawa, 2005) .... 87 Figure 7-4: Schematic of a nanorod growth process showing direct impingement of atoms on
Figure 7-7: Various atomic processes taking place on the surface ... 94 Figure 7-8: Depiction of the monomer flux and the diffusion flux of atoms (Markov, 1941) 98
Figure 9-1: Zones in the flame for various nanorod growth processes... 113 Figure 9-2: Variation of saturation pressure of MoO2 through the nanoparticle trajectory with
the growth timespan ... 115 Figure 9-3: Rate of nucleation for 0.75 mm and 1.00 mm molybdenum probes during the nucleation timespan ... 117
Figure 9-4: Variation of monomer partial pressure with the growth timespan ... 118 Figure 9-5: Variation of atomic flux on the growing nanorods with the growth timespan .. 119
Figure 9-6: Variation of length and diameter of nanorod from 1.00 mm diameter probe with the growth timespan ... 121 Figure 9-7: Variation of length and diameter of nanorod from 0.75 mm diameter probe with
growth timespan ... 123 Figure 9-8: Comparison of the contribution to the rate of increase in nanorod length by
surface diffusion and direct impingement with growth timespan ... 124 Figure 9-9: Trajectory followed by the nanoparticles from 1.00 mm and 0.75 mm probes during the growth timespan ... 126
Figure 9-10: Variation of aspect ratio of nanoparticles with monomer partial pressure ... 127 Figure 10-1: Solution of the Khrgian-Mazin size distribution, QMOM (solid), analytical
Figure 10-4: Variation of 1st moment during growth with growth timespan ... 155 Figure 10-5: Variation of higher moments for the nanorod size distribution with growth
Definition of Nanomaterial and One-Dimensional
Nanomaterials are defined as structures with dimensions that fall between the size range of 1 to 100 nm. This miniaturization of material is fairly new and thus has been the subject of
growing attention of modern science. Through successful efforts in this field many new opportunities can be realized especially pertaining to memory storage, electronics and computing. Nanomaterials are quite fascinating in many respects, mainly in the peculiar
properties that they exhibit. Owing to their extremely miniscule size the properties of nanostructures are considerably different from their bulk materials (Cao, 2004). For instance,
the melting temperature of many nanostructures has been found to be significantly less than the bulk material (sometimes by as much as 1000oC). Materials seem to lose their ferromagnetic behavior when reduced to nanoscale dimensions. Many of the properties of
is rather high and ensures that many constituent atoms are exposed on their surface. A keen interest in the production of nanoparticles was spurred by their display of some highly
desirable traits such as increased catalytic activity (Beck, et al., 1992), superplasticity (Karch, et al., 1987) and higher theoretical densities. The products manufactured with some
nanomaterials show higher toughness (Karch, et al., 1990) and ductility. One-dimensional nanostructures are commonly defined as nanoparticles with an aspect ratio greater than or equal to 3. One-dimensional nanostructures include a wide variety of products like whiskers,
fibers, nanowires and nanorods. Although whiskers and nanorods are generally considered shorter than nanowires and fibers. 1-D nanostructures, as generally accepted, provide a sound
basis to investigate the dependence of electrical and thermal transport on the dimensionality of nanostructures.
Figure 1-2: SEM images of ZnO nanobelts (Cao, 2004).
1-D nanostructures possess even higher surface to volume ratios making them perfectly suited to sensing and catalytic applications. Their surfaces have been modified to implement
them as highly sensitive, real time sensors for pH and biological species (Cui, et al., 2001). The charge on the surface of the particle changes as a result of the adsorption. Recently, (Kind, et al., 2002) found the conductance of ZnO nanowires to be extremely sensitive to
ultraviolet light exposure thus making it possible for them to make highly sensitive electrical switches.
Transition Metal Oxide Nanostructures
with an incomplete d sub-shell.” They are the elements occupying groups 3 to 12 on the periodic table.
Figure 1-3: Transition metals shown on the periodic table (Wikipedia, 2014)
Transition metals have unique properties because of their oxidation states. They form wide variety of colored compounds because of their electronic transitions from a ligand orbital to a
metal orbital when the metal is in a high oxidation state or from a metal to a ligand when the metal is in a low oxidation state. They also exhibit paramagnetic properties when they have
paramagnetic and the spin vectors are aligned parallel to each other (Figgis, et al., 1960). Owing to their oxidation states they can also make a plethora of ionic compounds.
When oxygen combines with transition metals it gives rise to many interesting properties. Silicon oxide and titanium oxide are used for biomolecule immobilization by exploiting their
large surface area (Zhuo, et al., 2005). Zirconium oxide is used for catalytic action due to its high surface energy (Xiao, et al., 2003). In recent years some effort has been devoted to the synthesis of molybdenum oxide due to its unique electronic and catalytic properties (Zhou, et
al., 2003). They have found tremendous use in petroleum refining and recording media (Song, et al., 2011) (He, et al., 2003).
Flame Synthesis of Nanoparticles
Flame synthesis has gained immense popularity as a method for producing nanoparticles.
The volumes of commercial flame production of nanoparticles has scaled to several million metric tons per annum with around 100 metric tons per day (Kammler, et al., 2001). The success and wide spread application of combustion synthesis is chiefly attributed to the
following advantages –
i. the heat of combustion easily activates precursor pyrolysis, hydrolysis and
ii. many parameters can be varied to control the final morphology of the nanoparticles iii. high heat allows the production of particles to be conducted under high purity
iv. flame processes can often be completed in a single step as compared to multiple steps in wet-chemical methods
v. flame methods are highly scalable
There are different configurations of flames that are used for nanoparticle synthesis. The
three basic type of burners are shown in Fig 1-4 .
Figure 1-4: Different burner configurations (a) premixed flat flame burner (b) counterflow
diffusion flame burner (c) coflow diffusion flame burner (Rosner, 2005)
Premixed flat flame burner
This kind of a burner configuration is used for oxide synthesis under sub-atmospheric conditions. The flow of fuel and oxidizer takes place either from the top or bottom to pass
over a vaporizing precursor. The flame is stabilized between the burner and a cooled substrate (Zhao, et al., 2005)
Counterflow diffusion flame burner
In a counterflow burner the particle precursor vapors are added either to the gaseous fuel or
the gaseous oxidizer. The end product is produced in the confined flame (Chung, et al., 1985) (Zachariah, et al., 1989) (Kim, et al., 2005)
Coflow diffusion flame burner
In a coflow burner the gaseous fuel and the oxidizer streams are separated from the stream carrying the precursor particles. This capability can be used to control the location of particle
inception in the flame (Zhu, et al., 1997).
1.3.1Steps in Flame Synthesis of Nanoparticles
The formation of nanoparticles involves a series of steps as depicted in Figure 1-5. The
building blocks of the nanoparticles are monomers. Monomers are distinctly identifiable particles having characteristic dimensions which come together to form clusters. Monomers are formed by the interaction of flame with the raw material introduced. Once the interaction
happens a series of chemical reactions occur converting the raw material into embryonic units. Some of these monomers polymerize to form nuclei which are the primary particles.
takes place on some existing nuclei without formation of new ones. This process is called heterogeneous nucleation. These nuclei then collide to form aggregates providing sites for heterogeneous deposition. The aggregates grow by surface deposition of monomers on these structures. When they are sufficiently large they may even undergo coalescence to form even
bigger structures thus giving them final shape. If the characteristic time for coalescence has the same order as the characteristic time for collision, branchy or hard aggregates are formed. All these processes are highly susceptible to variables like pressure, temperature and
Figure 1-5: Steps in particle formation in flames (Roth, 2007)
1.3.2Parameters Affecting Flame Synthesis
In the flame process nanoparticles are formed by gas-to-particle conversion mechanism. This mechanism has a characteristic of producing non-agglomerated particles. For production of a
for the purpose of experimental examination laminar flames are preferred as turbulence brings in other uncertainties. The process is affected by a number of parameters chiefly
temperature, particle residence time, precursor concentration and additives. Irrespective of the configuration of the flame the effect of these parameters remains rather unchanged. Other
variables like flame stoichiometry, gas flow rate etc. can be altered to control the particle morphology.
It has been observed that increasing precursor loading resulted in an increase in the particle
size. This effect has been attributed to increased agglomeration of the primary particles since the increase in precursor loading favors surface growth onto existing particles. The increased
collision frequency diminishes the available precursor concentration for any further homogeneous nucleation. The precursor loading also increased the density due to higher agglomeration. This surge in density provides more number of attachment points in the
particle and sintering occurs more rapidly. The precursor also affects the process temperature if a considerable amount of heat is provided by the combustion of the precursor increasing
the adiabatic flame temperature (Kammler, et al., 2001).
Flame temperature and particle residence time have been shown to be the most critical parameters in determining the particle morphology. An increase in temperature enhances the
precursor reactions thereby providing a boost to the monomer production but this also enhances the sintering process. Therefore an increase in temperature results in smaller
Burner geometry also plays a significant role in the process (Wegner, et al., 2002). Reducing the burner diameter by a quarter they were able to produce silica particles that were four
times smaller. This was the result of the enhanced mixing of gases in the smaller reactor which lead to a steeper temperature gradient. The smaller burner diameter also resulted in
higher outlet velocities thus reducing the residence time of the particle and consequently there is less time for their growth and sintering.
The particle size can also be controlled by using additives. These do affect the purity of the
product but can still be used to monitor the crystallinity and extent of agglomeration in the nanostructure. Small amounts of AlCl3 are infused to promote the formation of rutile titania
and to slow down the aggregation of the product (Braun, 1997). Stable and fully oxidized nanoparticles are normally obtained in flames burning under lean conditions. The oxygen stoichiometry in the particles depends on the distribution of oxygen concentration in the
flames. The stoichiometry of oxide particles affect their crystalline morphology and lattice structure. Many metals exist in various oxidation states and can form a variety of sub-oxides.
1.3.3Flame Synthesis of One-Dimensional Nanostructures
Limited work is available on flame synthesis of one-dimensional nanostructures as opposed to spherical nanostructures. These efforts include gas phase as well as solid support synthesis
to form nanorods especially Fe. The dimensions observed were 200 nm in length and 20 nm in diameter. Carrier gases also play a vital role.
ZnO nanorods have also been prepared by using flame spray pyrolysis in a coflow diffusion flame (Height, et al., 2006). Here too dopant species were used, primarily In, Sn and Li. The
formation of nanorods took place in the vapor phase and depends on the dopant valency. The nanorods produced were about 150 nm in diameter and 4 µm to 200 nm in length. Layer growth mechanism is responsible for this process. ZnO nanorods have also been prepared by
using oxygen microwave plasma torch flame (Hong, et al., 2006).
Numerical Modeling of Flame Synthesis of Nanoparticles
Flame methods for nanoparticle synthesis are quite complex and it is difficult to control their every aspect. This is one of the prime reasons that a perfect numerical simulation of
nanoparticle synthesis still remains elusive. In flame processes the chemical reaction and particle growth take place simultaneously and both are extremely fast processes. The complex fluid flow accompanied with short residence time makes it extremely difficult to
capture the physics (Pratsinis, 1998). Flame methods also contain a wide array of particle sizes and shapes which makes the particle characterization very difficult. The essence of
A literature review in the subject reveals various modeling strategies ranging from thermodynamics to stochastic methods and many other approaches that have been
undertaken. (Barnard, et al., 2005) has suggested a thermodynamic model to describe the shape of nanoparticle as a function of size and chemical environment. This model is based on
the concept of minimizing the total energy and hence used equilibrium thermodynamics. Although this model was able to successfully predict crystal structures but being based on equilibrium principles was unable to model kinetic growth of crystals. Kinetic models have
also been developed based on the assumption that under non-equilibrium conditions different crystal planes have different kinetic parameters (Xu, et al., 2007). Although these models
work whether the growth is in the solvent or the vapor phase, they are unable to take into account surface atomic processes. Flames contain polydisperse particles and non-spherical fractal structures for which non-spherical particle dynamic simulations and flame analysis
have not been carried out. The simulation of synthesis of fine titania done by (Johannessen, et al., 2000) employed a monodisperse model thus losing the effect of polydispersity.
Similarly, (Yu, et al., 1998) developed a discrete sectional model to be applied to flames but once again assumed spherical particles.
Population Balance Equation (PBE) has proved to be immensely helpful in modeling the
population of particles undergoing nucleation, coalescence and sintering. The PBE can either be univariate or bivariate depending on the requirements. Monodisperse models typically use
Another approach towards solving the PBE is Sectional Methods. They divide the entire distribution into bins and track the evolution of particles in each bin. Coupled differential
equations are formed together with the neighboring bin and the accuracy depends on the discretization schemes used. However, these techniques suffer from the problem of
numerical diffusion to neighboring bins. This problem can be solved by increasing the number of bins but that makes it computationally more expensive. These methods are easy to solve but run into high computational cost (Hounslow, et al., 1988).
Motivated by this, the work done in this thesis has been aimed at developing a numerical model which is able to predict the shape of non-spherical (typically one-dimensional
nanostructures) as they are grown in a flame environment in the gas phase. Due consideration has been given to the atomic processes taking place in each individual nanoparticle and also towards the collective dynamics of the entire group of particles undergoing morphological
changes in the flame volume (Srivastava, et al., 2014).
The goal of this thesis is to develop an innovative numerical scheme for simulating the growth of one-dimensional nanostructures in flames and to validate it using the results from
A counterflow flame has been simulated which interacts with the nanoparticles right from inception to final development. Detailed molybdenum surface oxidation chemistry has been
employed to simulate source precursor formation. Every development stage from nucleation to surface growth has been thoroughly examined along with flame-particle interaction and
particle transport. Results of the model have been compared to the experimental studies. A statistical analysis has also been performed on the synthesis process by using the Quadrature Method of Moments to study the collective characteristics of the group of nanoparticles.
Layout of the Thesis
Chapter 2 gives the experimental details of the Flame Gradient Method against which the
simulation results have been compared. Chapter 3 introduces the basics of growth mechanism of nanorods in flames followed by the subparts of the model in Chapters 4, 5, 6, 7
and 8. These chapters are Flame modeling, Monomer formation, Nucleation, Nanorod growth and Particle transport respectively. Together they form the entire nanorod growth mechanism. Chapter 9 discusses the results of the growth model and Chapter 10 explains the
An experimental study into the formation of one-dimensional molybdenum oxide
nanostructures has been carried out in the University of Oklahoma (Merchan-Merchan, et al., 2009). They explored the synthesis of transition metal oxide nanostructures produced in the
gas phase in oxy-methane flames through the Flame Gradient Method. More details can be found at (Desai, 2010). Their findings have been used to validate the numerical study undertaken in this research. For the purpose of providing an insight into the Flame Gradient
Figure 2-1: Schematic representation of the set-up (Desai, 2010).
In the Flame Gradient Method a counterflow flame is utilized to produce one-dimensional
nanostructures. The fuel used is 96% methane with 4% acetylene and the oxidizer utilized is 50% oxygen and 50% nitrogen. The fuel is introduced from the top nozzle whereas the oxidizer inlet is from the bottom nozzle. The two streams impinge onto each other to form an
opposed flow diffusion flame. The major advantage of a diffusion flame is the presence of high gradients of temperature and chemical species concentrations. Depending on the
is also an inlet of nitrogen from the outer annulus of the oxidizer nozzle. This layer of nitrogen is maintained to contain the diffusion flame and also to shield it from external air
effects. The nozzle separation is 25.4 mm and all experiments were performed at a strain rate of 20 s-1. Before combustion all the gasses are thoroughly mixed in the mixing chambers.
2.1.1Thermophoretic Sampling Technique
Figure 2-2: Thermophoretic sampling technique (Merchan-Merchan, et al., 2003)
Thermophoretic sampling technique is extensively used to capture particles in flame volume and has been applied in the study of soot formation (Megaridis, et al., 1988). Similar method
hence the growth of nanoparticles occurs rather quickly in a thin stretch of the flame. For this reason the thermophoretic sampling has to be extremely precise. The grid used here has a
copper mesh and has a thin film of 20 nm of pure carbon on one side. It is placed at an angle of 15o with plane perpendicular to the burner axis to minimize the travel time of the grid in
the particle formation area. Care should be taken while inserting the thermophoretic grid into the flame because of two main reasons.
i. The grid should not stay so long as to alter the flow of gases in the flame
ii. The duration of the sampling process should be long enough to capture the nanoparticle effectively.
The nanoparticles captured were analyzed using a high-resolution transmission electron microscopy (TEM) to analyze their structure and morphology.
2.1.2Effect of Oxidizer Composition on the Flame
The opposed flow diffusion flame is composed of two distinct regions – i. Blue zone – rich in oxygen atoms
ii. Yellow zone – rich in carbon atoms
For the synthesis of metal oxide nanostructures the molybdenum probe should be introduced into the blue zone. By varying the content of oxygen in the oxidizer the thickness of these
zones can be controlled.
Figure 2-3: Methane flames at a strain rate of 20 s-1 formed by a) 21% O2, 79% N2 b) 50%
O2, 50% N2 c) 100% O2 (Desai, 2010)
As can be seen from the Figure 2-3 21% O2 flame has a huge yellow zone whereas 100% O2 flame has a blue zone. On the other hand 50% O2 and 50% N2 has an ideal thickness of both
blue and yellow zone and hence this combination has been used in the experiments.
2.1.3Effect of Strain Rate on the Flame
At lower strain rates the yellow zone is most distinct and bright. This signifies an active carbon rich zone. As the strain rate increases the blue zone also increases in thickness but beyond a certain limit of strain rates the thickness of the blue zone again starts to recede.
Figure 2-4: Flames at various strain rates (35% O2 + 65% N2): (a) SR = 10 s-1(b) SR = 20 s -1(c) SR = 30 s-1 (Desai, 2010).
The Flame Gradient Method involves the production of nanomaterial through the interaction
of a metal in the form of a probe and the counter-flow flame. For molybdenum oxide nanoparticles molybdenum probes of different diameters act as the material source. Two probes of diameters 1.00 mm and 0.75 mm are used. These metal probes are inserted into the
flame at a distance of 13 mm from the fuel nozzle. In an oxy-methane counter-flow flame temperature gradients of 2000 K/cm exist along with steep chemical gradients. Due to this
the interaction of the probe with the flame is strongly affected by the probe position. The synthesized nanoparticles are sampled out using the thermophoretic technique at three levels in the flame volume (Z = 12mm, 11 mm, 10 mm) as measured from the fuel nozzle.
thermophoretic grid. Significant modifications occur in the transported nanomaterial and it forms nanoparticles of different morphologies depending on the ambient conditions in the
Figure 2-5: Schematic of probe position (Desai, 2010).
2.2.1Nanoparticle synthesis from 1.00 mm diameter molybdenum probe
Figure 2-6: Low resolution TEM image of nanoparticles collected at Z = 12 mm from the
fuel nozzle (Desai, 2010).
The figure shows a plethora of small particles along with some heavy nucleated particles. The size of the nucleated particles is less than 8 nm and they are invariably spherical in
Figure 2-7: TEM images of nanostructures obtained at Z = 10 mm from the fuel nozzle (Desai, 2010)
As the molybdenum oxide vapors travel through the flame they condense and undergo a
phase transformation to form solid nanoparticles. This phase change depends on the residence time of the particles which increases as the sampling height of the experiments
transformations (Figure 2-7). As compared to Figure 2-6 the nanostructures here have a more pronounced morphology. The structures are well-defined nanorods.
Figure 2-8: Magnified images of the nanoparticles sampled at Z = 10 mm (Desai, 2010). (a)
In order to thoroughly investigate the geometry of the structures the TEM grid is rotated to give a magnified view of the captured nanomaterial (Figure 2-8). Examination of these
images shows well faceted longitudinal particles with well-defined aspect ratios. Figure 2-8 (c) shows a nanorod with length ~100 nm and lateral dimension ~40 nm.
2.2.2Nanoparticle Synthesis from 0.75 mm Diameter Molybdenum Probe
Figure 2-9: Low resolution TEM image of nanoparticles formed by 0.75 mm probe at Z = 10
Figure 2-10: Magnified TEM images of nanoparticles formed by 0.75 mm probe (Desai,
Looking at Figure 2-9 it is evident that the number of particles formed are clearly much
higher than the ones formed when the 1.00 mm diameter probe was used as the material source. But there is a marked difference in their morphologies. The particles collected in
Figure 2-10 even at a distance of 10 mm all exhibit spherical geometries. There are no traces of any nanorods or polyhedral shaped nanoparticles. The largest particles are approximately 80 nm in diameter and the smallest are about 5 nm.
Conclusions of Experimental Results
Probes of different diameters (1.00 mm and 0.75 mm) were placed in the highly oxidative
conditions for the nanoparticles to grow in the flame volume. The variation in the probe diameter strongly affects the morphology of the resulting nanostructures. Experiments with
1.00 mm diameter probe yield well defined nanorods whereas the 0.75 mm diameter results in the synthesis of mainly spherical amorphous nanoparticles. For nanorods preferential
Brief Introduction to the
The mechanism of growth and morphology of nanoparticles is dictated by internal as well as external factors. It depends on the structure of the unit cell, defects in the crystal (internal
factors), the growth conditions and the type of synthesis method employed (external factors). The interplay of these external and internal factors is imperative to comprehend the
mechanism behind nanoparticle growth and predicting the texture and structure of the nanoparticles. During the growth of a nanoparticle various surface defects develop in the structure and along with impurity elements play an active role in determining the
morphology of the particle. The process of understanding their role leads to the development of methods of controlling perfection and homogeneity of nanostructures according to their
utility in the industry owing to their unique desirable qualities.
Nanoparticle formation begins only when a driving force perturbs the equilibrium of the system and a nucleus begins to grow. This growth can take place in any ambient condition
but their relative contribution is determined by the type of growth mode and the ambient conditions.
As will be seen later, the interface of a nanoparticle can be classified into atomically rough and smooth surfaces. The two types of surfaces have different type of growth modes and
eventually give rise to crystals having different morphologies. Nanoparticles formed under small driving force conditions will generally exhibit polyhedral forms as well as elongated structures like nanorods, whiskers, hollow tubes etc. Whether a nanoparticle is freely grown
or bounded by a substrate also affects the shape.
Heat and mass transfer being an important part of the growth process exert varying levels of
contribution depending on the ambient phase. For growth of particles in a dilute phase the mass transfer plays a greater role whereas for the growth in a condensed (liquid) phase heat transfer is of prime importance since the densities of the solid and melt phases don’t differ a
Finally, the entire process of nanoparticle growth is divided into three major steps –
i. A driving force in the form of a difference in the supersaturation levels provides the initial push for the supersaturated phase to condense into an aggregate state.
ii. Precursor atoms called monomers come together to form small clusters. Some of these clusters combine and grow larger than the critical size while the ones who are unable to overcome the critical size barrier wither away. This process is called
Details of the Growth Model
The entire mathematical scheme for simulating the development of one-dimensional nanorod
in the flame has been divided into two parts as shown in Figure 3-1 below
Figure 3-1: Subdivisions of the numerical model.
The Flame Model employs the open source software Cantera (Goodwin, 2009) to simulate the 1-D counter-flow diffusion flame. It solves for the species, mass, momentum and energy
however a one way coupling between the two sections. Information is passed from the Flame Model over to the Growth Model but no passage of information takes place from the Growth
Model to the Flame Model. This has been done with the assumption that the volume of nanoparticles created is extremely minuscule in comparison to the flame and there is no
change in the flow field due to the nanoparticles.
The Growth Model focuses on the development of a single nanorod and simulates its development through time in various conditions. Simulation of the entire group of
nanoparticles is the content of study for Chapter 10where the entire distribution of the nanorods produced in the flame has been studied.
In accordance with the experiments the numerical simulations have been carried out to understand the growth processes for two monomer sources –
i. 0.75 mm diameter molybdenum probe
ii. 1.00 mm diameter molybdenum probe
Nanorod formation is an extremely complicated process and entails several intricately related physical parameters. Being the first step towards the modeling of 1-D nanorods, this work
i. While calculating the temperature of the molybdenum probes the transfer of heat has been assumed to occur only through convection. The axial conduction has been
ii. Upon oxidation the molybdenum probes form molybdenum dioxide monomers. Since
the concentration of the monomers is considerably small they have been treated as an ideal gas and their concentration has been measured in terms of partial pressure. iii. The nucleation process has been modeled using the Classical Nucleation Theory. As a
result the assumptions of CNT have also been imbibed into the simulation. Hence in spite of the fact that the formed nuclei are suspended in the flame environment, the
properties of the molybdenum dioxide nuclei have been taken to be equal to that of the bulk material and the shapes of all the nuclei have been assumed to be spheres as is the case with liquid droplets.
iv. All the nanorods have been assumed to have developed from equal sized critical nuclei.
v. The growth of the nanorods only starts after the nucleation attains completion by reaching its maximum peak value.
vi. The growth on the lateral surfaces of the nanorods proceeds by 2-D nucleation which
give rise to single layers of atoms. Beyond a threshold this maturation should transcend into layered growth. However, instead of simulating the
vii. The distribution of various sizes of nanoparticles in a process develops due to differences in their growth times and growth rates. Although in the simulation all the
particles start their growth simultaneously, the Quadrature Method of Moments has been used to introduce moment methods into nanorod development so they can be
enhanced subsequently. To implement this study an initial distribution has been imposed by assuming a normal distribution of the particles with their mean size as the critical size of the nuclei and the standard deviation as the difference in the size
The Flame Gradient Method uses a one dimensional counter flow flame for the production of
1-D nanostructures. The fuel used is 96% methane and 4% acetylene along with the oxidizer which comprises of 50% oxygen and 50% nitrogen. The flame strain rate is 20 s-1. The flame
Figure 4-1: Schematic diagram of opposed flow diffusion flame.
Opposed Flow Flame Model
A counterflow flame configuration consists of two circular nozzles directed towards each other. The flow of oxidizer and fuel, coming from opposing directions, impinge and form a stationary flame. The location where the momentum of the two streams balance is known as
the Stagnation Plane which can be controlled by altering the flow rate of wither the fuel or the oxidizer mass flow rates. Since, as compared to the fuel more oxidizer is required by
This type of counter flow flame structure is especially suited to studies in nanoparticle formation for two reasons –
i. The flame is suspended freely in space, being completely free from burner heat losses and catalytic effects
ii. It is assumed that the flow properties are functions of axial distance only and the radial velocities vary linearly, thus essentially reducing the two dimensional flow into one-dimensional
A detailed derivation of the governing equations is given by (Kee, et al., 1988) but a short
summary of these equations is given below.
The mass conservation equation in cylindrical coordinates –
x r r
where 𝑢 and 𝑣 are the axial and radial velocity components and 𝜌 is the density. Two dimensional flow has been reduced here to a one dimensional description by assuming the
fluid properties to be dependent only on the axial direction and a linear variation of the radial properties with the radial distance. Equation (4.1) is satisfied by stream function
, ( )
x r r U x
v G x
F x equation (4.1) reduces to
Since G and F are functions of x only so now the temperature, density, velocity and mass fractions all become functions of x only.
Introducing the above mentioned assumptions into the Navier Stokes equation it becomes
clear that 1/r
are functions of x alone. Since
x r r r r x
Therefore, for the radial momentum equation
1 p H r r constant 2 3
2 d FG G d d G 0
dx dx dx
pk k k k k
p p p
dT d dT dT
u C Y V h
dx C dx dx C dx C
k k k k
u Y V W
The diffusion velocities can either be given in the multi-component form
1 K j kT 1
k j kj j
dX D dT
V W D
X W dx Y T dx
or in the mixture-averaged form
1 k kT 1
dX D dT
X dx Y T dx
40 where / K j j j k km K j jk j k X M D
M X D
Y is the mass fraction, Cpis the specific heat, hkis the species molar enthalpy, Wkis the
species molar mass and kis the chemical production rate, is the viscosity and is the
D , Dkmand DkTare the binary diffusion, mixture averaged and thermal diffusion coefficient
Generally the temperature, mixture composition and the inlet velocity are specified at the
inlet and the symmetry conditions are applied at the stagnation plane. Equations (4.1) to (4.6) form a boundary value problem.
Solving the above equations requires the knowledge of transport properties like diffusion
coefficients, viscosities, thermal conductivities and thermal diffusion coefficients (Kee, et al., 1986). The transport properties can be calculated either in mixture averaged or
multicomponent fashion. Mixture averaged properties carry the advantage of simplicity and low computational expense but they also have the following disadvantages –
i. Accuracy – The mixture averaged quantities are accurate only for simple cases as
ii. Mass conservation – Mixture averaged method does not necessarily ensure overall conservation of mass in the species conservation equation.
4.2.1Mixture Averaged Properties
A short summary of the procedures followed by any standard combustion simulation code to calculate the mixture averaged transport properties is given here. For more detailed
explanations and for procedures to calculate multicomponent transport properties refer (Kee, et al., 1986).To calculate the mixture averaged or multicomponent properties the transport
properties of pure species must first be known. Polynomial fits are generated for the temperature dependent part of the pure species properties. This ensures the absence of any redundancy in calculating the collision integrals and other expensive operations. Their
expressions have been summarized below (Hirschfelder, et al., 1954) Viscosity – 2 5 16 k B k k
W k T
where k is the Lennard-Jones collision diameter, mk is the molecular mass, kB is the
Boltzmann constant. The collision integral depends on the reduced temperature and the reduced dipole moment.
Binary diffusion coefficients –
where mjk is the reduced molecular mass and jk is the reduced collision diameter. In
considering the reduced quantities care should be taken whether the molecules are polar or non-polar.
Mixture averaged diffusion coefficient for species k –
/ K j j j k km K j jk j k X M D
M X D
Mixture averaged viscosity –
1 1 K k k K k j kj j X X
(4.10) where 2
1 1 1
2 2 4
1 1 1 8 j k k kj
j j k
M M M M
Mixture averaged thermal conductivity –
1 1 1 1 2 / K
k k K k k k k X X
The flow equations contain convective and diffusive terms. The discretization technique
followed is a non-uniform grid where upwind differencing is used for convective terms and central differencing for diffusive terms. The upwind scheme ensures better convergence and has a first order approximation whereas the central differencing gives a second-order error
The initial grid can be defined by the user or it can be generated automatically with the initial
number of grid points being chosen by the user. The above equations, applied at each point of the grid form two point boundary value problems. TWOPNT (Grcar, 1992) solver program is used to solve these steady state system of equations.
GRI-Mech 3.0 (Smith, et al.) provides all the relevant information for describing the
combustion of methane and natural gas including NO formation and reburn chemistry. It involves 325 elementary chemical reactions of 53 species and has been validated for all the
major steps in the combustion process deriving from the knowledge of reaction rate theory. The mechanism has been optimized for a temperature range of 1000 K to 2500 K, pressures of 10 Torr to 10 atm and equivalence ratios of 0.1 to 5 for premixed systems. Certain
However, it does not incorporate certain aspects of methane combustion like soot formation and the chemistry behind selective non-catalytic reduction of NO. In spite of its lack of
optimization for ethane, propane, methanol, ethylene and acetylene it has been incredibly successful as a combustion mechanism. GRI mechanism was originally developed for
methane combustion but its applicability for acetylene has been established by comparison with the Warnatz mechanism (Movileanu, et al., 2012).
Results of the Flame Model
Counter-flow diffusion flames possess large gradients of temperature and chemical species concentrations. These gradients constitute the prime advantage of the Flame Gradient
Method over other synthesis techniques to study the formation mechanism of nanoparticles. Depending on the required material and the characteristics of the nanoparticle product
various zones of the counter-flow flame can be utilized. Figure 4-2 shows the chemical species profiles in the opposed flow oxy-methane flame. The flow equations have been solved using Cantera (Goodwin, 2009). Fuel used in these simulations is the same as the one
used in the experiments (96% CH4 + 4% C2H2) and the oxidizer used is also same as the one used in the experiments (50% O2 + 50% N2). The distance between the nozzles is 25.4 mm
and the strain rate is 20 s-1.The plot shows the fuel nozzle on the left side and the oxidizer nozzle on the right side with all the distances being measured from the fuel inlet. Methane and oxygen are at their highest concentrations at their nozzle inlets respectively and decrease
45 i. oxygen rich zone
ii. carbon rich zone
For producing metal oxide nanoparticles the raw material is introduced into the oxygen rich zone which instantly oxidizes the metal in the hot environment to form metal oxide
precursors. Conversely, for producing carbon nanorods the raw material is placed in the carbon rich zone of the flame. Acetylene concentrations also follow similar trends as the methane concentration. Addition of acetylene has a marked effect on the temperature of the
flame. A minute quantity of 4% of acetylene causes the temperature to rise by about 40oC which provides a conducive atmosphere for the molybdenum oxide nanorods to grow.
Figure 4-4: Gas velocity as a function of axial position.
Figure 4-3 and Figure 4-4 give the details of the temperature and the gas velocity. The
maximum temperature of 2780oC results near the 13 mm mark from the fuel nozzle. The gas velocity is also plotted as a function of distance. Negative values of velocity signify the
from the fuel nozzle. The inlet gas velocities have been calculated from the strain rate equation.
2 . . U S R
Monomers are the basic building units of complex molecules and structures. They bind with
each other chemically to give rise to larger crystal shapes. In the case of molybdenum oxide nanorods the monomers are single molecules of MoO2 which undergo different attachment
patterns to form different shapes under varying conditions of supersaturation ratio.
In a nutshell the mechanism of monomer formation is as follows. When the probe is introduced into the oxygen rich zone of the flame it gets oxidized forming MoO3. MoO3
being extremely volatile starts to move up with the flame and as it approaches the fuel nozzle the reducing atmosphere converts the MoO3 to MoO2, forming the monomers. To completely comprehend the monomer formation and its implications on the growth of nanostructures a
monomer formation model has been developed which incorporates a molybdenum oxidation mechanism. The information on amount of molybdenum oxidized also provides the
Commercial interest in molybdenum is particularly high due to its ability to withstand high
temperatures. It has a melting point of above 2000 K hence making it ideal for applications in furnaces and high speed, high temperature flight. It also possesses considerable strength at high temperatures as compared to other common metals. However, molybdenum is highly
susceptible to oxidation and the rate of oxidation continues to increase with temperature until the metal loses all its use. This severely reduces the lifespan of the metal component and
restricts its functionality. The oxidation behavior of molybdenum has been studied (Douglass, 1970) (Kubaschewski, et al., 1967) and in oxidizing atmosphere molybdenum starts to sublime above 500oC. The reaction of molybdenum with oxygen is complex and
from room temperature to 1700oC involves a number of different oxidation processes (Saburi, et al., 2001).
A number of studies have been dedicated to understand the complicated phenomena of molybdenum oxidation since it has different oxidation regimes under different temperature conditions. Under the temperature limit of 400oC adherent oxide layers were observed on the
surface of the metal (Gorbounova, et al., 1956). The oxidation rate data was fitted under a parabolic curve and energy of activation of 36 kcal/mole was determined. Considerable
deviations to this parabolic law were observed over 400oC with volatilization occurring at 475oC under vacuum conditions. When the pressure was increased to 1 atm the vaporization temperature changed to 650oC. (Simnad, et al., 1955) observed the behavior between 500oC
above 500oC. However, catastrophic oxidation set in at 725oC (Lustman, 1950). (Peterson, et al., 1954) investigated the oxidation of molybdenum at higher temperatures as a function of
temperature and pressure and found that it followed a linear rate law at all temperatures and pressures thus indicating that a non-protective oxide was formed.
Another interesting aspect to the oxidation process is the transport phenomena. To include the effects of transport (Bartlett, et al., 1958) conducted experimental studies with the reaction system in air between 760oC and 1204oC using a flow system. The flow rate was
found to affect the rate of oxidation which slowly increased with the temperature as well as the flow rate.
Oxidation Regimes of Molybdenum
(Gulbransen, et al., 1963) conducted a detailed study into the oxidation regimes of
molybdenum, its chemical mechanism and the rate controlling factors. Since under certain conditions molybdenum forms both oxide scale and volatile molybdenum trioxide therefore a) it was essential to determine the nature of the reaction b) the kinetics of oxidation was
studied over a wide temperature and pressure range to study the primary chemical reaction c) it was essential to ascertain the transition zone between chemical and transport controlled
oxidation. They considered the following five reactions with the listed standard free energies of reaction and equilibrium pressures–
Mo + O2 ↔ MoO2, ΔFo kcal/mole (R1)
2MoO3 ↔ 2MoO2 + O2 PO2 atm (R3)
3MoO2 ↔ 2MoO3 + Mo ΔFo kcal (R4)
nMoO3 ↔ (MoO3)n at 600oC, n = 3.24 (R5)
Table 5-1: Thermochemical data for Oxides of Molybdenum
298 - 127.45 -159.7 5.38 x 10-48 + 63.0
400 - 122.9 -153.45 4.44 x 10-34 + 61.85
600 - 114.1 - 141.35 1.42 x 10-20 + 59.6
800 - 105.55 - 129.6 7.23 x 10-14 + 57.45
1000 - 97.15 - 118.1 7.10 x 10-10 + 55.3
1200 - 88.95 - 112.7 9.51 x 10-8 + 50.4
1400 - 80.95 - 108.25 1.56 x 10-6 + 43.7
1600 - 73.05 - 99.55 ---- ----
1800 - 65.35 ---- ---- ----
They observed that pressure had little effect on the reaction below 800oC but beyond that limit the effect of pressure on the reaction rate was large and the rate followed the 1.5 power
of the pressure. Oxidation studies too showed similar phenomena. The percentage of oxygen forming oxide scales reduces with temperature. At 700oC only 30% of the oxygen is
employed in the formation of scales. Molybdenum metal is oxidized forming three layers: the outermost MoO3, the innermost MoO2 and the intermediate layer which can be expressed by MoxO3x-1 (Mo4O11, Mo8O23, Mo9O26). At 800oC however, all of the oxygen used forms
volatile molybdenum trioxide at atmospheric pressure. They concluded that between 600oC and 800oC both solid oxide and volatile oxide occur. But above 800oC only volatile
molybdenum trioxide is formed. The various oxidation regimes of molybdenum can be summarized as follows –
Table 5-2: Classification scheme; oxidation of molybdenum (Gulbransen et. al., 1963)
Oxidation Process Rate controlling
1 Below 450oC Adherent oxide films or scales form
Diffusion of metal or oxygen through oxide
2 500o – 700oC Oxide scales form also oxide volatizes
Oxide scales not protective. Chemical type processes on metal surface
3 801oC to
Liquid oxide can form, volatizes as soon as oxide forms
55 Table 5-2 Continued
4 Above transition temperature
Oxide volatizes as fast as it forms
Transport of oxygen to metal interface. Turbulence in gas is important
In the Flame Gradient Method the temperature of molybdenum oxidation is always greater
than the transition temperature hence the mode of oxidation always has transport of oxygen as the critical factor.
Mechanism of Molybdenum Oxidation
The entire process of oxidation of molybdenum comprises of five major steps (Jones, et al., 1958)–
i. transport of oxygen to the surface ii. chemisorptions of the oxygen
iii. chemical reaction at the surface iv. desorption
v. transport of reaction products
The slowest of these is the rate controlling step. Processes ii, iii and iv are chemical processes and are marked by a large activation energy whereas processes i and v are transport processes